The Microstructure Characterization and the Mechanical ...cdn. The Microstructure Characterization
Embed Size (px)
Transcript of The Microstructure Characterization and the Mechanical ...cdn. The Microstructure Characterization
The Microstructure Characterization and the Mechanical Properties of Electrospun
Chen Zhang, Xuejia Ding and Sizhu Wu Key Laboratory of carbon fiber and functional polymers, Ministry of Education,
College of Materials Science & Engineering, Beijing University of Chemical Technology, Beijing,
Electrospinning provides a straightforward and cost-effective approach to produce fibers from polymer solutions or melts having the diameters ranging from sub-microns to nanometers (Reneker & Chun 1996 ; Dzenis 2004; Hammel et al. 2004; Greine & Wendorff 2007). The nanofiber fabrication by the electrospinning technique can also provides high orientation of the polymer chains by some special colleting accessories due to the high elongation forces that developed during the electrospinning process. This process is accompanied by massive solvent evaporation which leads to fibers with high packaging density(Doshi & Reneker 1995). The carbon fibers possess high mechanical strengths and moduli, superior stiffness, excellent thermal and electrical conductivities, as well as strong fatigue and corrosion resistance; therefore carbon nanofibers have recently received increased attention for their potential applications as composite reinforcing fillers, heat-management materials, high-temperature catalysts, membrane-based separation media, and components in nanoelectronics and photonics etc.(Chand 2000). There are several precursors for the production of carbon fiber, such as polyacrylonitrile (PAN), pitch and cellulose(Edie 1998; Basova et al. 2004) etc. But PAN is the most widely used precursor for manufacturing high-performance fibers due to its combination of tensile and compressive properties as well as its high carbon yield(Sutasinpromprae et al. 2006). Usually, the PAN or PAN-based carbon fiber is produced by the following steps: (1) first, spinning the precursor under different drawing ratio, (2) then, the precursor fiber is stabilized at 200 to ca. 300C in an oxidation atmosphere; (3) finally, the stabilized fiber is heated at temperatures from 1200 to ca. 3000 C in an inert atmosphere to wipe off nearly all of the non-carbon element to obtain the final carbon fibers. There are two critical factors in these manufacturing processes of PAN carbon fibers which one is to control the suitable orientation and crystallization of the precursors and the other is the post-treatment steps such as pre-oxidization, stabilization and carbonization. Conventional PAN-based carbon fibers typically have diameters ranging from 5 to 10 um (Morgan 2005). However, the electrospun PAN nanofibers are uniform with the diameters of approximately 300 nm (Chun et al. 1999; MacDiarmid et al. 2001), which is more than 30 times smaller than their conventional counterparts. The high specific surface
Nanofibers Production, Properties and Functional Applications
area of electrospun polymer and carbon nanofibers leads to the enhanced properties in various applications such as electrodes in fuel cells and supercapacitors. The subsequent thermal treatments, including pre-oxidization, stabilization and carbonization, convert the PAN precursor nanofibers into carbon nanofibers that are very long (continuous) probably with desired microstructural, electrical, mechanical, and other properties. However, the mechanical properties of electrospun nanofibers need to be improved because of the limited crystallinity and orientation during the electrospinning (Li et al. 2003). The microstructures and the related mechanical and/or electrical properties of the electrospun carbon nanofibers are still largely unknown. Carbon nanotubes (CNTs) have achieved a momentous research and application interest due to their unique properties, such as high tensile modulus, good heat and electrical conduction, unique optical and electronic properties, and so forth. It is found that reinforcement of polymers by CNTs may significantly improve their mechanical properties, thermal stability, electric conductivity, and other functional properties. For enhancing the properties of the nanofibers, the carbon nanotubes (CNTs) have also tried to introduce in the PAN-based composites due to their appealing mechanical (Wong et al. 1997; Yu et al. 2000), electrical (Javey et al. 2003), and thermal conductivity properties (Miaudet et al. 2007). Both single-walled carbon nanotubes (SWNTs) and multiwalled carbon nanotubes (MWNTs) are of scientific interest in nanotechnology and nanodevices because of their superior structural, mechanical, chemical, thermal, and electrical performance(Iijima 1991; Baughman et al. 2002; Collins et al. 2001). The SWNT reinforced pitch-based carbon microfibers(Andrews et al. 1999) and PAN/CNTs microfibers(Sreekumar et al. 2004) exhibited a significant improvement in mechanical properties and thermal stability. It has been shown that significant interactions exist between PAN chains and CNTs, which lead to higher orientation of PAN chains during the heating process (Rilutsky et al. 2010). It is also shown that CNTs embeds in electrospun PAN nanofiber serve as nucleation centers for graphitic structure formation during the carbonization process leading to a more ordered and oriented structure. For pre-oxidization, stabilization and carbonization, it is noteworthy that applying tension during thermal treatments, particularly during stabilization, is crucial for the development of carbon fibers with high mechanical strength; i.e., if the stabilization is carried out without tension, the resulting carbon fibers are mechanically weak (Donnet et al. 1998; Morgan 2005). However, before full realization of their reinforcing improvement, the following two crucial issues have to be solved: (i) dispersion and orientation of CNTs in the nanofiber (Chandrasekar et al. 2009; Hao et al. 2006), good interfacial bonding is required to achieve load transfer across the CNTs-matrix interface (Chen et al. 2006); (ii) the macroscopic alignment in the nanofibers (Na et al. 2009) and the orientation and crystallinity of polymer chains. Therefore, in this chapter, the manufacturing process and characterization methods for the microstructures and mechanical properties of PAN and PAN-based nanofibers has been reviewed.
2. Manufacturing and characterization of the PAN and CNTs/PAN composites nanofibers
2.1 Manufacturing of the PAN and PAN-based nanofibers The PAN and PAN-based nanofibers can be made by electrospinning with the nominal electric field on the order of 1 kV/cm. Fig.1 is the schematic diagram of the electrospinning technique. In the process the PAN or CNTs/PAN solution is held by its surface tension at
The Microstructure Characterization and the Mechanical Properties of Electrospun Polyacrylonitrile-Based Nanofibers
the end of a capillary, such as a stainless steel needle. As the intensity of the electric field is increased, usually by increasing the voltage, the hemispherical surface of the solution at the tip of the capillary tube elongates to form a structure named as a Taylor cone (Taylor 1969). At a certain voltage the electrical forces overcome the surface tension and a jet ejects from the Taylor cone. The jet travels some distance and then a whipping instability begins to further attenuate the jet into nanofibers. The fibers are collected onto a counter electrode, such as a screen, drum, plate, or the edge of a rotating disk. Coupled with the usual observations the fact that fibers can be electrospun using an Ac field indicates that a portion of the attenuation occurs in the stable jet region. The Dc electrospun fibers are smaller than Ac spun fibers indicates further drawing occurs in the instability region. The voltage between the electrode and the counter electrode could be controlled by the high voltage power supply such as setting at 14-16 kV. The collector rotated at some surface speed such as 6.6m/s, which the high speed rotating collector could align the nanofibers into the nanofiber sheets.
Fig. 1. Schematic diagram of the electrospinning technique.
Since N,N-dimethylformamide(DMF) is the common solvent of PAN-based carbon fibers manufacturing process which can easily evaporate during the electrospinning, the DMF can be selected as solvent and are through mild bath sonication to have a completely dissolution. Usually the suitable weight concentration of PAN/DMF can be selected higher than 10% with the PAN average molecular weight of 100,000 g/mol. Fig. 2 shows the SEM micrographs of different concentrations of electrospinning PAN/DMF solutions of 8 wt %, 10 wt % and 12 wt % respectively. At the 8 wt% PAN/DMF ratio (Fig. 2A), viscous forces
Nanofibers Production, Properties and Functional Applications
within the jet are insufficient to stabilize disturbances, leading to capillary breakup. At 10 wt% and 12 wt% PAN/DMF ratios, irregular and regular beads formed, respectively (Fig. 2B,C). Therefore it can be said as the PAN/DMF ratio increases higher than 10wt%, viscous forces stabilize disturbances at the jet surface, leading to a beads-onstring configuration. However, if the concentration was too high, controlling and maintaining a stable flow rate becomes very difficult because the viscosity of the polymer solution is high.
Fig. 2. SEM micrographs of PAN/DMF different concentrations of electrospinning nanofibers with the solutions of (A)8 wt %; (B)10 wt %; (C)12 wt %.
To uniformly disperse the CNTs in the organic polymer matrix, the CNTs are modified to form an individually polymer-wrapped structure(Waclawik et al. 2006). As is well known, polymer wrapped greatly inhibits the Van der Waals attraction between the po